Building a robust 3D Ca-MOF by a new square Ca<sub>4</sub>O SBU for purification of natural gas.
Hu, Falu; Di, Zhengyi; Wu, Mingyan; Li, Jing; Dalton transactions (Cambridge, England : 2003) 49 (2020) 8836–8840; doi:10.1039/d0dt00943a

data_7704591
_publ_section_title
;
 Building a robust 3D Ca-MOF by a new square Ca<sub>4</sub>O SBU for
 purification of natural gas.
;
_journal_issue                   26
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              8836
_journal_page_last               8840
_journal_paper_doi               10.1039/d0dt00943a
_journal_volume                  49
_journal_year                    2020
_chemical_formula_sum            'C8.25 H7 Ca0.5 O2.62'
_chemical_formula_weight         168.17
_space_group_crystal_system      tetragonal
_space_group_IT_number           87
_space_group_name_Hall           '-I 4'
_space_group_name_H-M_alt        'I 4/m'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2016/6
_audit_update_record
;
2020-02-12 deposited with the CCDC.	2020-06-02 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   13.8229(11)
_cell_length_b                   13.8229(11)
_cell_length_c                   24.906(2)
_cell_measurement_reflns_used    14024
_cell_measurement_temperature    110(2)
_cell_measurement_theta_max      72.40
_cell_measurement_theta_min      4.52
_cell_volume                     4758.9(7)
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_diffrn_ambient_temperature      110(2)
_diffrn_measured_fraction_theta_full 0.986
_diffrn_measured_fraction_theta_max 0.983
_diffrn_measurement_device_type  'Bruker SMART APEX2 area detector'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0354
_diffrn_reflns_av_unetI/netI     0.0255
_diffrn_reflns_Laue_measured_fraction_full 0.986
_diffrn_reflns_Laue_measured_fraction_max 0.983
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       30
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_number            13991
_diffrn_reflns_point_group_measured_fraction_full 0.986
_diffrn_reflns_point_group_measured_fraction_max 0.983
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         72.396
_diffrn_reflns_theta_min         5.754
_exptl_absorpt_coefficient_mu    2.419
_exptl_absorpt_correction_T_max  0.7536
_exptl_absorpt_correction_T_min  0.6478
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
 SADABS 2016/2: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    0.936
_exptl_crystal_description       block
_exptl_crystal_F_000             1392
_refine_diff_density_max         0.942
_refine_diff_density_min         -0.630
_refine_diff_density_rms         0.077
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.091
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     119
_refine_ls_number_reflns         2380
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.091
_refine_ls_R_factor_all          0.0765
_refine_ls_R_factor_gt           0.0734
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1601P)^2^+4.5869P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2335
_refine_ls_wR_factor_ref         0.2387
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2197
_reflns_number_total             2380
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0dt00943a2.cif
_cod_data_source_block           F:data_I
_cod_depositor_comments          'Adding full bibliography for 7704591.cif.'
_cod_original_cell_volume        4758.9(9)
_cod_original_formula_sum        'C8.25 H7.00 Ca0.50 O2.62'
_cod_database_code               7704591
_shelx_shelxl_version_number     2016/6
_shelx_res_checksum              34750
_shelx_fab_checksum              39959